Polymer 97 (2016) 63e68
Contents lists available at ScienceDirect
Polymer journal homepage: www.elsevier.com/locate/polymer
Effect of the naphthenic oil and precipitated silica on the crystallization of ultrahigh-molecular-weight polyethylene Fulchiron a, * Fabien Toquet a, Laurent Guy b, Brice Schlegel b, Philippe Cassagnau a, Rene a b
Univ Lyon, Universit e Claude Bernard Lyon 1, CNRS UMR 5223, Ing enierie des Mat eriaux Polym eres, F-69622 Villeurbanne Cedex, France Solvay Silica, 15 rue Pierre Pays BP52, 69660 Collonges au Mont d’Or, France
a r t i c l e i n f o
a b s t r a c t
Article history: Received 8 March 2016 Accepted 6 May 2016 Available online 9 May 2016
Ultrahigh molecular weight polyethylene (UHMW-PE) belongs to the specialty polymer grade because of its unique properties. Among other applications, it is used for battery separator membranes elaboration for automotive applications. These PE separators are porous membranes composed of a blend of UHMWPE, naphthenic oil and precipitated silica. With the aim of understanding the membrane structuring mechanisms, we studied the inﬂuence of silica and oil concentrations on the UHMW-PE crystallization during the elaboration process. Results have shown that the high initial thickness of the UHMW-PE crystals is reduced after the process. Moreover, cc (crystallinity) and Tc (crystallization temperature) are both controlled by the volume fraction of oil. The initial high crystallinity of UHMW-PE (cc z 65%) can be increased in the membrane with a high Oil/PE ratio. Furthermore, silica indirectly contributes to enhance the UHMW-PE crystallinity by acting as a reservoir, hence increasing the possible oil content in the blend. © 2016 Elsevier Ltd. All rights reserved.
Keywords: Ultra high molecular weight polyethylene Naphthenic oil Silica
1. Introduction Ultrahigh molecular weight polyethylene (UHMW-PE) belongs to the specialty polymer grade because of its unique properties of good chemical resistance, impact strength and abrasion resistance [1e3]. UHMW-PE due to its ultra-high molecular weight (Mw > 1.0 106 g.mol1) has a very high viscosity at the melting state. Thus UHMW-PE is generally processed by sintering the nascent powder , which keeps the high crystallinity (z65%) of the nascent powder in the ﬁnal material . However for some UHMW-PE transformation like spinning [5e7] or porous membrane elaboration [8e10] it is necessary to proceed the UHMW-PE in dilute system. An application of this UHMW-PE porous membrane is separator for lead-acid battery. Separator is an important component of a lead-acid battery which must keep the cathode and the anode apart to avoid the shutdown. Separators made with UHMW-PE, precipitated silica and naphthenic oil are called PEseparator . Nowadays, this separator represents more than 90% of the worldwide lead-acid battery separator market . PEseparator popularity is due to its excellent microporous structure
* Corresponding author. E-mail address: [email protected]
(R. Fulchiron). http://dx.doi.org/10.1016/j.polymer.2016.05.021 0032-3861/© 2016 Elsevier Ltd. All rights reserved.
for electrolyte ﬂow, its good chemical resistance as well as its excellent mechanicals properties (ductility, strength, puncture resistance and toughness for envelopability) [8,12]. Most of these properties are improved by the use of UHMW-PE instead of HDPE or LDPE . In the PE-separator industry, PE-separator are manufactured by passing the components (UHMW-PE, precipitated silica and process oil) through a heated extruder, the extrudate is then calendared and, after cooling, a part of the oil is extracted from the membrane by the use of solvent [3,13,14]. This kind of process is known by Thermally Induced Phase Separation (TIPS) process . A polymer (UHMW-PE) and a diluent (process oil) are blended at a sufﬁciently high temperature to obtain a homogeneous phase, after cooling, the process oil is no longer a diluent for the polymer. By removing the oil, the porosity required for battery separator application is obtained. The interaction between polymer and diluent is a key parameter in controlling the ﬁnal morphology of the membranes in TIPS process . Polymer/diluent interaction parameter for PE/parafﬁn blends has been widely investigated [17e20] but the PE/naphthenic oil interaction parameter is not well described in the literature and will be discussed in this article. The crystallization kinetics of UHMW-PE during TIPS process or the use of surfactant on the crystallization have been well studied  as well as the effect of doped silica on HDPE crystallization. LI et al. observed that the addition in excess of PEG into UHMW-PE/diluent
F. Toquet et al. / Polymer 97 (2016) 63e68
blend induces a lower PE crystallinity . Zhang et al. observed that the addition of silica in HDPE/diluent blend leads to a crystallinity variation from 45% to 50% without no obvious trend with the addition of doped silica . In this study, the effects of the addition of precipitated silica and the dilution of UHMW-PE into oil on the UHMW-PE crystallization (melting and crystallization temperature as well as crystallinity) have been investigated with a view of understanding the role of the oil quantity. The effect of silica and oil on HDPE and L-LDPE were also studied as comparison systems to understand the speciﬁcity of the UHMW-PE crystallization behavior. 2. Experimental 2.1. Materials
2.3. Thermogravimetric analysis (TGA) In order to accurately determine the actual quantity of each material in the used DSC pans, these were perforated before proceeding to thermogravimetric analyses. A TGA Q500 TA Instrument was used. Samples were heated from 30 C up to 550 C at a heating rate of 8 C/min. Thus, the amounts of polyethylene (PEwt%), Oil (Oilwt%) and silica (Silicawt%) were obtained. 2.4. Determination of polyethylene’s crystallinity In order to determine the melting enthalpy corresponding to the polyethylene into the blend (DHmPE), TGA results are used to normalize the melting enthalpy of the blend obtained by DSC, by the amount of polyethylene:
Three kinds of polyethylene were used in this study. The UHMW-PE (GUR®4150) with M w ¼ 9 106 g.mol1 was kindly supplied by Ticona. The HDPE (HDT10) with M w ¼ 105 g.mol1 and ÐM ¼ 3.2 was provided by Haldia Petrochemicals Limited. The LLDPE (TM50-U) with M w ¼ 8 104 g.mol1 and ÐM ¼ 2.5 was supplied by SNETOR. The naphthenic Oil, Shell Edelex Oil 946, was supplied by Shell. The precipitated silica powder Zeosil® 1165 with D50 ¼ 19.4 mm and a speciﬁc BET surface of 149 m2/g was supplied by Solvay. By adding drop by drop the oil to the precipitated silica and mixing them by hand until exudation, we estimate the oil absorption capacity of the Zeosil® 1165 at 312 ml/100 g for the Shell Edelex Oil 946.
2.1.1. Preparations of samples For this study, for distinguishing the effect of oil and silica, we used two kinds of samples: PE/Oil blends and PE/Oil/Silica blends. However, this approach led us to process differently for both samples kinds because of their different ﬂow behaviors.
First of all, it is important to notice that the Oil/PE ratio in the process samples is not necessarily equal to the setpoint after process. In fact, during the process at 165 C, PE and naphthenic oil are described as miscible , but after cooling, due to the phase separation, a loss of oil by exudation can happen. However, as shown in Fig. 1, precipitated silica helps to avoid the oil exudation during and after the process. From a mass ratio Si/PE of 2, the initial Oil/PE ratio of 7.5 (represented with a dashed line in Fig. 1) is maintained whereas without silica the Oil/PE ratio after process is only 2.3. Due to its porous structure, the use of silica as ﬁller to prevent exudation in blends is helpful. In these formulations, silica is crucial to keep all the oil inside the blend during and after cooling. Obviously for a higher desired amount of oil, necessary precipitated silica quantity should be higher. Fig. 2 shows typical DSC results for the studied blends. In Fig. 2a, which corresponds to the re-crystallization after
2.1.2. PE/Oil blends (suspension samples) Homogeneous PE/Oil blends were simply prepared in a mortar at room temperature, leading to suspensions of polyethylene powder into naphthenic oil. The PE powders were mixed to the Oil with a volume fraction of Oil (4Oil) ranging from 0 to 0.9. 2.1.3. PE/Oil/Silica blends (process samples) Homogeneous PE/Oil/Silica blends were prepared in an internal mixer (Haake™ Rheomix) with roller rotors. The samples were prepared at 165 C with a rolling speed of 60 rpm during 12 min with a ﬁlling factor of 80%. The blends were then cooled at room temperature. The Si/PE mass ratio varies from 0 to 3 while the Oil/ PE ratio was ﬁxed to 7.5 for all these blends with silica.
The polyethylene crystallinity in the blend is calculated by the following equation with the assumption that the heat of fusion (DHf0 ) of the purely crystalline polyethylene is 293 J/g :
3. Result and discussion
2.2. Differential Scanning Calorimetry (DSC) Crystallization studies were carried out using a Pyris Diamond DSC instrument (Perkin Elmer). The sample was ﬁrst heated from 30 C up to 165 C at a heating rate of 20 C/min and maintained at this temperature for 2 min. This step is crucial for erasing and controlling the thermal history. Then, the sample was cooled down to 30 C at a cooling rate of 10 C/min in order to characterize the crystallization. Thereafter, the crystallization temperature (TC) will be considered at the peak onset. Finally the sample was again heated up to 165 C at 20 C/min in order to obtain the melting enthalpy values of the blend (DHmBlend) and the corresponding melting temperature (Tm) which will be taken at the peak maximum.
Fig. 1. Variation of Oil/PE weight ratio after process as a function of Silica/PE weight ratio inside the blend (dashed line is the oil/PE ratio before process).
F. Toquet et al. / Polymer 97 (2016) 63e68
Fig. 2. Example of DSC results: a) First cooling curves b) Second heating curves.
the ﬁrst melting, the crystallization temperature is shifted to lower temperatures when increasing the Oil/PE ratio. In the same way, as it can be seen in Fig. 2b, Tm is also shifted to lower temperature with the increase of Oil/PE ratio. The melting temperatures of all studied samples are presented in Fig. 3 as a function of their respective Oil/PE ratio. From Fig. 3 we can notice that, for each of the three PE in blends, Tm decreases with increasing oil content, independently of the blending process and the presence or not of silica. Moreover, the lower melting temperature observed for L-LDPE is directly linked to its lower attainable crystal thickness due to the higher branches content [24,25]. Furthermore, as we can see in Fig. 3, samples with or without silica are on the same trend, hence the amount of the silica appears to have no effect on the Tm diminution. Therefore, it is reasonable to consider that this Tm diminution is only connected to the PE dilution into naphthenic oil. From this viewpoint, it is legitimate to analyze the results in the framework of the Flory-Huggins theory  from which the following relation between the equilibrium melting point and the dilution is derived:
1 0 Tm;Eq
RVu 4d c42d Dhu Vd
0 where Tm,Eq and Tm;Eq are the equilibrium melting temperatures of
respectively the polymer in solution and the bulk polymer 0 (Tm;Eq ¼ 414:6 K) and Vd is the molar volume of the diluent, Vu is the molar volume of the repeat unit, DHu is the heat of fusion of the repeat unit (4096 J.mol1), 4d is the volume fraction of the diluent in the blend (here the naphthenic oil) and c is the Flory-Huggins interaction parameter. An interaction parameter value lower than 0.5 indicates a total miscibility while the miscibility is only partial for c greater than 0.5 . However, in Eq. (3) the equilibrium melting temperatures are very fastidious to determine for each dilution. Therefore, it is convenient to modify this equation using the Gibbs-Thomson equation which relates the actual melting point and the crystalline lamella thickness (L):
Tm ¼ Tm;Eq 1
DHf0 rc L
where rc is the crystal density (0.997 g.cm3) and s ¼ 8.3 102 J.m2 is the speciﬁc surface energy of the crystalline lamella which remains quasi independent of the diluent . Considering now that, for a given studied PE, and because of the same cooling process for all the samples, the obtained crystalline lamellae are approximately of the same thicknesses L, the bracket in Eq. (4) can be considered as nearly constant . Therefore, Eq. (3) becomes:
1 1 RVu 0 ¼ 4Oil c42Oil Tm Tm ð1 AÞ Dhu Vd
with: A ¼ DH20sr L c f In the present case, only the binary blend of PE and oil has to be taken into account for expressing 4Oil because the silica is an inert phase. Hence, 4Oil is obtained from the volume content of PE (VPE) and the volume content of Oil (Voil) as described in equation (6).
Fig. 3. Melting temperature as a function of Oil/PE weight ratio after process.
VOil Voil þ VPE
From Eq. (5), it is obvious that the plot of 1/Tm,Eq versus 4Oil should be quadratic with a curvature linked to the interaction parameter value. These types of plot shown in Fig. 4 for L-LDPE, HDPE and UHMW-PE, exhibit quasi linear evolutions (only very slight curvatures might be distinguished but much lower than for c ¼ 0.5). Therefore, the interaction parameter can be considered very close to 0 which is favorable for the dissolution. For
F. Toquet et al. / Polymer 97 (2016) 63e68
Fig. 4. Inverse of melting temperature as a function of FOIL (Lines serve as guide for eyes, dashed line for c ¼ 0 and solid line for c ¼ 0.5 in Eq. (5)).
comparison, it can be mentioned that, for PE/parafﬁn blends analogous to the blends studied in the present work, Chen and Wolcott obtained an interaction parameter of approximately 0.06 for PE . As a result of the nature of the naphthenic oil, which is a blend of parafﬁns, naphthenes and aromatics , it is not possible to give an exact value of Vd. However, we can estimate an equivalent molar volume of the diluent by considering the slope values of the plots in Fig. 4 that correspond to the prefactor of Eq. (5). It must be pointed out that, using the parameters values previously given; the constant A varies only from 0.033 for HDPE and UHMW-PE to 0.047 for LLDPE. Thus, the ratio Vd/Vu is estimated from the slope values between 1.11 104 K1 and 1.12 104 K1. Hence, a ratio of z19 is obtained indicating that the equivalent molar volume of the diluent can be considered 19 times larger than the repeating unit volume of PE (eCH2e). It can be concluded that, despite the several assumptions made to estimate this ratio, the obtained value appears quite consistent regarding the oil nature. Concerning the crystallization analysis, in Fig. 5, the crystallization temperatures of all studied samples are presented as a
Fig. 5. Crystallization temperature as a function of 4Oil.
function of their respective 4Oil. Once again, for the three types of polyethylene, TC decreases with the increase of oil content. The variation of TC for the samples with UHMW-PE, HDPE and L-LDPE are respectively from 124 C to 107 C, from 121 C to 106 C and from 114 to 100 C. Basically, TC decreased of about 15 C for each polyethylenes. Because the cooling rate is the same for all experiments, it can be considered in a ﬁrst approximation that, the crystallization likely occur for similar quench depth (difference between the melting temperature in the polymer-oil blend and the actual temperature). Consequently this decrease of TC is linked to the phase diagram of PE/Oil and the Tm,Eq decreasing when increasing 4Oil [20,29]. This decrease of TC for UHMW-PE was already observed for UHMW-PE/Liquid Parafﬁn blend (LP) by Zhang et al. . As concerns the material properties after processing, it is obvious that the PE crystallinity obtained will be a crucial parameter. From our experiments, this crystallinity is analyzed on the basis of the second heating DSC curves (Fig. 2b). This crystallinity is obtained after renormalization of the peak enthalpies using Eq. (1) to take into account the PE content in the DSC sample. Then, the PE crystallinity is calculated from Eq. (2). Fig. 6 shows the obtained crystallinity as a function of 4Oil for all samples. For the HDPE and the L-LDPE, there is absolutely no effect of the dilution into oil on their respective crystallinity. The samples of HDPE and L-LDPE have a crystallinity around 62.5% and 43.5% respectively. As expected, L-LDPE exhibits the lowest crystallinity due to the branches on the polymer chain [24,25]. Chen and Wolcott also observed that the dilution of HDPE in parafﬁn does not affect their crystallinity in HDPE/Parafﬁn but they observed a slight diminution of crystallinity for L-LDPE/Parafﬁn blend . However, for the UHMW-PE samples, there is obviously an inﬂuence of the dilution on the resulting polymer crystallinity. Indeed, for UHMWPE the crystallinity drastically increases from 40 to 65% with the increase of oil content. This phenomenon is attributed to the ability of the solvent to provide the necessary mobility to the polymer chains leading to a more perfect crystallization. This necessary mobility is enough without diluent for classical melt PE (HDPE and LLDPE) but for the very long chains of UHMW-PE, the effect of the diluent is manifest. Process and suspension samples with or without silica are on the same trend which means that the crystallinity of UHMW-PE is directly governed by 4Oil regardless the presence of silica or the processing means. Although, by permitting
Fig. 6. Crystallinity of polyethylene as a function of Foil .
F. Toquet et al. / Polymer 97 (2016) 63e68
higher content of oil in the blends for process samples, the precipitated silica permits to achieve indirectly a higher crystallinity than without silica. Indeed, due to its ability to absorb a large quantity of oil, the silica can retain this oil inside the material at ambient temperature while it is rejected by the PE itself because of the phase separation. In other words, the exudation of oil by the material at ambient temperature is avoided in presence of the silica. Therefore, during the process at high temperature and the following cooling, this excess of oil advantageously permits a more complete crystallization by providing even more mobility to the UHMW-PE macromolecules. In this respect, it can be added that the initial crystallinity of the nascent powder of GUR®4150 (UHMWPE) determined by DSC was about 65%. However, after one melting/ recrystallization, the UHMW-PE crystallinity decreases to 40% as it can be observed in Fig. 7. This diminution of crystallinity after melting is commonly reported for pure UHMW-PE [4,31,32]. Indeed, the chain topology of nascent UHMW-PE powder is at low level of entanglements due to the crystallization of individual chains during the polymerization which prevents entanglement with neighbor chains [33,34]. Nevertheless, at the melt state, a reentanglement occurs that generates a lower crystallinity after cooling . On the other hand, the dilution into oil makes it possible to exceed or, at least, to recover the initial crystallinity of the nascent powder. As a matter of fact, at the molten state, the UHMW-PE is soluble in the naphthenic oil which leads to the diminution of chains entanglement [29,30]. Park et al. have found that the entanglement molecular weight decreased linearly as a function of the UHMW-PE weight fraction . This diminution of chain entanglement induces a better mobility of UHMW-PE chains and a faster crystallization . Thus for a same cooling rate, this will lead to an increase of the crystallinity as shown in Fig. 6. However, there is no effect of dilution in oil on HDPE and L-LDPE crystallinity since the chain’s mobility of pure PE is already sufﬁcient to obtain the maximum crystallinity at 10 C/min cooling rate. In summary, diluting UHMW-PE into naphthenic oil increases the chains mobility of UHMW-PE and leads to an increase of its crystallinity. However in order to keep all the oil in the blend during the process, a minimum amount of silica is required. Finally, the amount of silica indirectly controls the UHMW-PE crystallinity by allowing a greater efﬁciency of the Oil/PE ratio in the blend during
Fig. 7. DSC curves for nascent powder of UHMW-PE: 1) 1st heating; 2) 1st cooling; 3) 2nd heating.
the process. 4. Conclusion Formulation of UHMW-PE/Oil/Silica blend prepared by thermally induced phase separation is crucial to control the crystallinity and the properties of the material. For the intended application, this is of primary importance because the crystallinity inﬂuences the durability of the PE-separator membrane. The results of the present study indicate that the amount of precipitated silica helps to keep naphthenic oil inside the UHMW-PE/Oil/Silica blend during the TIPS process and to avoid exudation after cooling at room temperature. Moreover, UHMW-PE crystallinity is controlled by the amount of oil present in the blend. With the increase of the Oil content there is an increase of UHMW-PE crystallinity which permits to, at least, recover the initial crystallinity UHMW-PE nascent powder. This increase of crystallinity due to naphthenic oil and precipitated silica should have, in term of application of the material as a battery separator, a beneﬁcial impact on the oxidation resistance in a sulfuric acid environment and the effect on the mechanical properties of the separator should be notable. To conclude, this study shows that the Si/PE ratio and the Oil content are both governing factors. They both permit to increase the crystallinity of UHMW-PE, the Oil content directly by providing mobility to UHMW-PE chains and Si/PE ratio indirectly by maintaining higher oil content in the blend. Acknowledgements The authors gratefully acknowledge Solvay group for the ﬁnancial support and providing the precipitated silica for this work. The authors would like to thank also the ANRT for its ﬁnancial support (CIFRE N 2013/0453). References  S.M. Kurtz, UHMWPE Biomaterials Handbook: Ultra High Molecular Weight Polyethylene in Total Joint Replacement and Medical Devices, Academic Press, 2009.  A.J. Peacock, Handbook of Polyethylene: Structures, Properties, and Applications, Marcel Dekker, New York, 2000.  T. Wada, T. Hirashima, J. Power Sources 107 (2002) 201e210. s, O. Lame, G. Vigier, F. Dore , Polymer 48 (2007) 6374e6383.  D. Jauffre  H. Matsuyama, H. Okafuji, T. Maki, M. Teramoto, N. Kubota, J. Membr. Sci. 223 (2003) 119e126.  N. Li, C.F. Xiao, Ira Polym. J. 18 (2009) 479e489.  Y. Wang, R. Cheng, L. Liang, Y. Wang, Compos. Sci. Technol. 65 (2005) 793e797.  L.C. Wang, M.K. Harvey, J.C. Ng, U. Scheunemann, J. Power Sources 73 (1998) 74e77.  S. Liu, W. Yu, C. Zhou, Polymer 55 (2014) 2113e2124.  S. Liu, C. Zhou, W. Yu, J. Membr. Sci. 379 (2011) 268e278. €hnstedt, J. Power Sources 133 (2004) 59e66.  W. Bo € hnstedt, J. Boesler, K. Ihmels, J. Power Sources 158 (2006)  J. Deiters, W. Bo 1069e1072.  P. Arora, Z. (John) Zhang, Chem. Rev. 104 (2004) 4419e4462.  H. Winkler, J. Power Sources 113 (2003) 396e399.  N. Li, C. Xiao, Z. Zhang, J. Appl. Polym. Sci. 117 (2010) 720e728.  D.R. Lloyd, K.E. Kinzer, H.S. Tseng, J. Membr. Sci. 52 (1990) 239e261.  A. Nakajima, F. Hamada, Kolloid-Z. Z. Für Polym. 205 (1965) 55e61.  C.M. Cormier, B. Wunderlich, J. Polym. Sci. Part -2 Polym. Phys. 4 (1966) 666e667.  A.Y. Coran, C.E. Anagnostopoulos, J. Polym. Sci. 57 (1962) 13e23.  F. Chen, M.P. Wolcott, Eur. Polym. J. 52 (2014) 44e52.  C.-F. Zhang, Y.-X. Bai, J. Gu, Y.-P. Sun, J. Appl. Polym. Sci. 122 (2011) 2442e2448.  C. Zhang, Y. Xia, K. Zuo, Y.-P. Zeng, J. Appl. Polym. Sci. 131 (2014) (n/aen/a).  B. Wunderlich, Thermal Analysis of Polymeric Materials, Springer, Berlin, 2005.  J. Fatou, C. Marco, L. Mandelkern, Polymer 31 (1990) 890e898.  F. Bustos, P. Cassagnau, R. Fulchiron, J. Polym. Sci. Part B Polym. Phys. 44 (2006) 1597e1607.  P.J. Flory, Principles of Polymer Chemistry, Cornell University Press, 1953.  U. Gedde, Polymer Physics, Chapman & Hall, London, 1995.
68     
F. Toquet et al. / Polymer 97 (2016) 63e68 Technical Data Sheet Shell Edelex Oil 946, n.d. S.S. Kim, D.R. Lloyd, Polymer 33 (1992) 1036e1046. C. Zhang, B. Zhu, G. Ji, Y. Xu, J. Appl. Polym. Sci. 99 (2006) 2782e2788. P. Gao, Man Ken Cheung, T.Y. Leung, Polymer 37 (1996) 3265e3272. T. Deplancke, O. Lame, F. Rousset, R. Seguela, G. Vigier, Macromolecules 48
(2015) 5328e5338.  B.P. Rotzinger, H.D. Chanzy, P. Smith, Polymer 30 (1989) 1814e1819.  Y.L. Joo, O.H. Han, H.-K. Lee, J.K. Song, Polymer 41 (2000) 1355e1368.  J.W. Park, J. Yoon, J. Cha, H.S. Lee, J. Rheol. 59 (2015) 1173e1189.